3 Study of Silicon Lg = 3-nm Bulk IM, AC, and JL FinFET
Tải bản đầy đủ - 0trang
282
8
Extremely Scaled Si and Ge to Lg = 3 nm FinFETs …
G
Fh
Top width (Fwt )
S
Bot. width (Fwb)
D
L g(nm)
28nm
20nm
12nm
9nm
EOT(nm)
0.5
0.5
0.3
0.3
Fh(nm)
46-60
46-60
50
50
Fwt (nm)
2-6
2-6
3
3
B
o
d
Y
Fwb(nm)
12
12
5
5
S/D Dop.
8E19
8E19
8E19
8E19
W= 20nm
H= 80nm
Ch. Dop.
8E18
8E18
5E18
5E18
Fig. 8.1 Device structure and parameters of simulated wine-bottle FinFET, with Fin height (Fh),
top Fin width (Fwt), and bottom Fin width (Fwb)
Figure 8.4 shows simulated linear Ids–Vgs sub-20-nm FinFET plots versus (a) Fh
and (b) Fwt. The Ids is highly depending on Fwt rather than Fh. The ion increases
with the Fwt increasing.
Figure 8.5 shows simulated linear Ids–Vgs curve of wine-bottle FinFET keep the
trapezoidal Fin of (a) pFET and (b) nFET. The results reveal that the Ion can be
increased (+18%) by using tall Fh and wide top Fin width (Fwt).
Figure 8.6 shows simulated 3D contour plot influence of Fh and Fwt for
sub-20-nm wine-bottle nFinET and pFinET with Vth, Ion, and Ioff, respectively. The
Vth and SS (not shown) are all reasonable and insensitive values (Vth < 14 mV,
SS < 3 mV/dec). The ion increases with Fin height (Fh), top Fin weight (Fwt)
increases monotonically, and Ioff is in opposite trend. Once achieving the target Vth
and Ioff values, the Ion can be increased by using larger Fwt.
Figure 8.7 shows simulated 3D contour plot influence of Fh and Fw for
Lg = 20-nm wine-bottle nFinET and pFinET with Vth, Ion, and Ioff, respectively. The
Vth and SS are all reasonable and insensitive values (DVth < 8 mV,
DSS < 4 mV/dec). The Vth insensitivity reveals that the Vtn and Vtp can entirely
adjust by using proper metal gate materials with different work functions. The Ion
increases with Fin height (Fh), top Fin weight (Fwt) increases monotonically, and
Ioff is in opposite trend.
Figure 8.8a plots the simulated timing characteristics of a Si CMOS inverter
circuit of simulated Lg = 12-nm wine-bottle FinFETs. The Thl is 0.89 ps, and Tlh is
1.8 ps. Figure 8.8b plots simulated SRAM characteristics with signal noise margin
(SNM) of 160 mV.
8.3 Study of Silicon Lg = 3 nm Bulk IM, AC …
283
Electron & Hole Density (oﬀ state)
STD
Tall, Fh(+13%), Fwb(-10%)
nFinFET
L g =28nm
Tall, Fh(+13%), Fwb(-10%)
STD
pFinFET
L g =28nm
Fig. 8.2 Simulation results of electron and hole density at off-state of (a) sub-20 nm n-type and
(b) p-type FinFET. The tall FinFET has lower electron and hole density distribution than STD
FinFET
8.3
Study of Silicon Lg = 3-nm Bulk IM, AC, and JL
FinFET
Methods are taken to reduce short-channel effects in traditional modes of operation
such as inversion-mode (IM). In future, they may be replaced by other new modes
of operation such as junctionless-mode (JL) of operation which is being researched
widely nowadays. To obtain higher on-state current (Ion), JL transistors are heavily
doped which leads to adverse effects on transport properties due to severe impurity
scattering. Research study on standard IM and JL FinFETs shows that ultra-scaled
FinFETs are inherently more sensitive to variability than standard devices and will
pose signiﬁcant challenges in post-CMOS technology. This chapter begins with the
brief introduction to the challenges posed in the sub-10-nm technology. A general
introduction about materials of current technology and prospective technology is
analyzed by considering the industrial trend. The operation of device in sub-10-nm
284
8
Extremely Scaled Si and Ge to Lg = 3 nm FinFETs …
(a) 10-4
(b) 10
-5
10
10
Vd =0.8V
Vd =-0.8V
-6
10
-7
10
10
-8
10
Vd =-0.05V
SS~64
-9
10
Vd =0.05V
SS~62
-10
10
10
10
10
-11
L g=28nm
EOT=0.5nm
Vg =0.8V
Fh=50nm
Fwt=6nm
Fwb=12nm
10
-12
10
10
10
-13
10
Ids (A)
Ids (A)
10
-0.8
-0.4
0.0
0.4
0.8
10
-4
-5
Vd =-0.7V
-6
-7
-8
-9
Vd =-0.05V
SS~68
-11
-12
-13
-0.8
-0.4
10
Ids (A)
10
10
10
10
10
10
10
-5
10
-6
10
-7
-8
10
Vd =0.05V
SS~68
Vd =-0.05V
SS~84
-9
-10
-11
-12
Lg=12nm
EOT=0.3nm
Vg=0.6V
10
10
10
-13
-0.8
10
10
Fh=50nm
Fwt=3nm
Fwb=5nm
-0.4
0.0
Vgs (V)
0.0
(d) 10 -4
Ids (A)
10
L g=20nm
EOT=0.5nm
Vg =0.7V
Fh=50nm
Fwt=6nm
Fwb=12nm
0.4
0.8
Vgs (V)
Vd =0.6V
Vd =-0.6V
Vd =0.05V
~67
-10
Vgs (V)
(c) 10-4
Vd =0.7V
0.4
0.8
10
-5
Vd =0.5V
Vd =-0.5V
-6
-7
-8
Vd =-0.05V
SS~86
Vd =0.05V
SS~75
-9
-10
-11
-12
Fh=50nm
Fwt=3nm
Fwb=5nm
Lg=9nm
EOT=0.3nm
Vg=0.5V
-13
-0.8
-0.4
0.0
0.4
Vgs(V)
0.8
Fig. 8.3 Simulated Ids–Vgs of (a) Lg = 28 nm, (b) Lg = 20 nm, (c) Lg = 12 nm, and
(d) Lg = 9 nm wine-bottle FinFET
node will be completely different from that of the devices in higher technology
nodes. The sub-10-nm technology devices will be more strictly adhering to the laws
of quantum physics and important quantum conﬁnement phenomenon, and
size-dependent properties will come to effect more severely in sub-10-nm node.
Hence, it is important to compare and analyze the performance of the conventional
inversion-mode of operation along with the other modes of operation such as
accumulation-mode and junctionless-mode. We examine the performance of the
optimized 3-nm FinFET with homogeneous source and drain doping concentration
in inversion-mode (IM), accumulation-mode (AC), and junctionless-mode
(JL) operation. The transfer and output characteristics in IM, AC, and JL modes
of simulated sub-5-nm technology node devices are discussed in detail. In addition,
8.3 Study of Silicon Lg = 3 nm Bulk IM, AC …
(b)
5x10-6
Fh=60nm
Fh=58nm
Fh=56nm
Fh=54nm
Fh=52nm
Fh=50nm
Fh=48nm
Fh=46nm
Ids (A)
4x10-6
3x10-6
2x10-6
Vd=-0.8V
Vd=0.8V
0.0
Fwt =5nm
Fwt =4nm
Fwt =3nm
Fwt =2nm
3x10-6
1x10-6
0.4
0
0.8
Vd=0.8V
Vd=-0.8V
2x10-6
Fwt=4nm
Fwb=12nm
-0.4
Fwt =6nm
4x10-6
1x10-6
0
-0.8
6x10-6
5x10-6
Ids (A)
(a)
285
Fh =50nm
Fwb=12nm
-0.8
-0.4
Vgs (V)
0.0
0.4
0.8
Vgs (V)
Fig. 8.4 Linear Ids–Vgs sub-20-nm FinFET plots versus (a) Fh and (b) Fwt. The Ids is highly
increasing with the Fwt
Ids (A)
4x10
3x10
2x10
1x10
(b) 6x10-6
-6
-6
-6
5x10
-6
4x10
-6
Ids (A)
(a) 5x10
-6
-6
3x10
-6
2x10
-6
0
Top/Bot Fw= 6/14 nm
Top/Bot Fw= 4/12 nm
Top/Bot Fw= 2/10 nm
-0.8 -0.7 -0.6 -0.5 -0.4 -0.3 -0.2
Vgs (V)
-6
1x10
0
0.3
Top/Bot Fw=6/14 nm
Top/Bot Fw=4/12 nm
Top/Bot Fw=2/10 nm
0.4
0.5
0.6
0.7
0.8
Vgs (V)
Fig. 8.5 Linear Ids–Vgs sub-20-nm FinFET trapezoidal Fin of (a) pFET and (b) nFET
for each case, we interpret the 3D electron density mesh plots. The device performances such as the drain-induced barrier lowering, subthreshold slope, and
on/off current ratio have also been estimated. This chapter serves as only a design
guideline and in future with more ab initio and ﬁrst principle-based models can be
incorporated in the device physics for more accurate results.
In this section, we investigated the device performance of the optimized 3-nm
gate length (Lg) bulk silicon FinFET device using 3D quantum transport device
simulation. By keeping source and drain doping constant and by varying only the
channel doping, the simulated device is made to operate in three different modes
such as inversion-mode (IM), accumulation-mode (AC), and junctionless-mode
(JL). The excellent electrical characteristics of the 3-nm gate length Si-based bulk
FinFET device were investigated. The subthreshold slope values
(SS * 65 mV/dec) and drain-induced barrier lowering (DIBL < 17 mV/V) are
analyzed in all three IM, AC, and JL modes of bulk FinFET with |Vth| * 0.31 V.
286
8
Extremely Scaled Si and Ge to Lg = 3 nm FinFETs …
Fig. 8.6 (a–c) are 3D plots of Lg = 28-nm nFET with Vth, Ion, and Ioff. (d–f) are 3D plots of pFET
with Vth, Ion, and Ioff, respectively. The Fwb is ﬁxed at 12 nm
Fig. 8.7 (a–c) are 3D plots of Lg = 20-nm nFinET with Vth, Ion, and Ioff, respectively. (d–f) are
3D plots of pFET with Vth, Ion, and Ioff, respectively. Fwb is ﬁxed at 12 nm
Furthermore, the threshold voltage (Vth) of the bulk FinFET can be easily tuned by
varying the work function (WK). This research reveals that Moore’s law can
continue up to 3-nm nodes.
The simulated device structure and the table of important parameters used in the
device simulation are given in Fig. 8.9. We applied equivalent oxide thickness
(EOT) of 0.3 nm. The gate length (Lg) is 3 nm, and the Fin width (Fw) and the Fin
8.3 Study of Silicon Lg = 3 nm Bulk IM, AC …
Voltage (V)
0.8
0.6
0.4
THL=0.89ps
0.2
TLH=1.8ps
0.0
-0.2
0
2e-11
4e-11
6e-11
8e-11
(b)
0.6
V
/V
(V)
out1 out 2
(a) 1.0
287
0.5
0.4
SNM=160mV
0.3
0.2
0.1
0.0
0.0
0.1
Time (s)
0.2
0.3
0.4
0.5
0.6
Vout2 / Vin1 ( V )
Fig. 8.8 Simulated Lg = 12-nm FinFET (a) inverter timing characteristics and (b) SRAM
characteristics with signal noise margin (SNM) of 160 mV
height (Fh) are also the same (Fw = Fh = 3 nm). The doping concentrations of
source/drain in all three modes (IM, AC, JL) of bulk FinFET devices are set to
1.0 Â 1020 cm−3 for both n-type and p-type transistors. The channel concentration
of JL bulk FinFET is set to 1.0 Â 1020 cm−3. The channel concentration of IM and
AC bulk FinFET is set to 1.0 Â 1018 cm−3. Arsenic and boron are used as dopants
in device simulation. The bulk doping concentration for the FinFET is
5 Â 1018 cm−3, which can be implemented easily by usual well doping implantation. A constant Vth value was maintained for both nFET (Vth * 0.31 V) and pFET
(Vth * −0.31 V) in all three modes of operation. The work function used for
n-type IM, AC, and JL modes is 4.40, 4.41, and 4.55 eV, respectively. Similarly,
the work function for p-type IM, AC, and JL modes is 4.80, 4.81, and 4.69 eV,
respectively. Precise numerical results of the simulated nanoscale device are
obtained by solving 3D quantum transport equations provided by Synopsys
Sentaurus version 2014. In quantum transport equations, a density-gradient model
is used in the simulation. The bandgap narrowing model and Shockley–Read–Hall
recombination with doping-dependent model are also considered. The mobility
model used in device simulation is according to Matthiessen’s rule.
RSRH ¼
np À n2i;eff
sp n ỵ n1 ị ỵ sn p ỵ p1 ị
8:1ị
Rsrh is the carrier composite item of Shockley–Read–Hall; sp and sn are lifetimes
of electrons and holes; ni,eff is the effective intrinsic concentration; and n1 and p1 are
constants of defect charge.
p ¼ Nv F1=2 ð
EF;p À Ev À Kp
Þ
kTp
ð8:2Þ
288
Extremely Scaled Si and Ge to Lg = 3 nm FinFETs …
8
Lg = 3nm
EOT = 0.3nm
h
w
Z
X
STI
Device Mode
Source & Drain
Doping
Concentration
Channel Doping
Concentration
Substrate Doping
Concentration
Junctionless
N : 1x1020 cm-3
P : 1x1020 cm-3
N : 5x1018 cm-3 ,P-Type
P : 5x1018 cm-3 ,N-Type
Y
Accumulation
Inversion
N :1x1020 cm-3
P :1x1020 cm-3
N :1x1020 cm-3
P :1x1020 cm-3
N : 1x1018 cm-3 ,N-Type
P : 1x1018 cm-3 ,P-Type
N : 1x1018 cm-3 ,P-Type
P : 1x1018 cm-3 ,N-Type
N : 5x1018 cm-3 ,P-Type
P : 5x1018 cm-3 ,N-Type
N : 5x1018 cm-3 ,P-Type
P : 5x1018 cm-3 ,N-Type
Fig. 8.9 Device structure and important parameters of simulated 3-nm gate length (Lg) IM, AC,
and JL Si bulk FinFET [3]
n ¼ Nc F1=2 ð
EF;n À Ec À Kn
Þ
kT n
ð8:3Þ
p and n are concentrations of hole and electron, respectively; F1/2 is Fermi–Dirac
integral; Nc and Nv are effective densities of states of conduction band and valence
band, respectively; and Tp and Tn are temperatures of hole and electron.
Kp ẳ
ch2
1
r2 ln p ỵ r ln pị2
2
12mp
8:4ị
Kn ẳ
ch2
1
r2 ln n ỵ r ln nÞ2
2
12mn
ð8:5Þ
mp and mn are effective mass of hole and electron, respectively, and Etrap is the
difference between defect energy level and intrinsic energy level. In addition, the
mobility model in the device simulation is in accordance with the following
Matthiessen’s rule:
8.3 Study of Silicon Lg = 3 nm Bulk IM, AC
1
D
ẳ
l lsurf
ỵ
aps
289
D
lsurf
ỵ
rs
1
lbulk
8:6ị
dop
In D = exp(x/lcrit), x is the distance from the interface, and lcrit is the ﬁtting
parameter. The mobility is composed of three kinds of phenomena, such as acoustic
phonon scattering (lsurf_aps), surface roughness scattering (lsurf_rs), and bulk
mobility with doping-dependent modiﬁcation (lbulk_dop).
Results and Discussion
Left-hand side plots of Figs. 8.10, 8.11, and 8.12 show the Id–Vg curves of the
n-type and p-type devices of interest, in which the linear threshold voltage (Vth) is
all adjusted to approximately ±300 mV for fair comparison. In the proposed n-type
IM, AC, and JL bulk FinFET, the saturation current (at Vg = 0.7 V, Vd = 1 V) is
2.52 Â 10−4 A/µm, 2.54 Â 10−4 A/µm, and 2.32 Â 10−4 A/µm, respectively. For
p-type IM, AC, and JL bulk FinFET, the saturation current is 2.24 Â 10−4,
2.25 Â 10−4, and 2.26 Â 10−4 A/µm, respectively. The SS for n-type IM, AC, and
JL modes is, respectively, 78.74, 78.79, and 77.37 mV/dec. The SS for p-type IM,
AC, and JL modes is 67.63, 67.65, and 62.28 mV/dec, respectively. The DIBL,
deﬁned as the difference in Vth between Vd = 0.05 V and Vd = 0. 7 V, for n-type
IM, AC, and JL modes, equals only 16.04, 16.17, and 26.80 mV/V, respectively.
The similar performances are also achieved in p-type IM, AC, and JL bulk
FinFET (29.80, 31.89 mV/V, and 40.20 mV/V). The DIBL and SS numerical values
are tabulated in Table 8.1. As the Fw and Fh are reduced to 3 nm, the SS and DIBL
approach to their ideal value (60 mV/dec and 0 mV/V) in the simulated results.
10
10
10
10
10
10
Si nFET
Si pFET
-3
Vds =-0.7V
0.5
Vds = 0.7V
-4
-5
Vds =-0.05V
JL Mode
Lg =3nm
Vds =0.05V
-6
-7
-8
-9
Si pFET SS :
62.28 mV/dec
Si nFET SS :
77.37 mV/dec
Si pFET DIBL :
40.20 mv/V
Si nFET DIBL :
26.80mv/V
-10
10
-1.0
-0.5
0.0
0.5
Gate Voltage (V)
IVg
Drain Current (mA/µ m)
Drain Current (A/ µ m)
10
1.0
0.4
Vth I= 0.4 V to 0.8 V
Step = 0.2 V
Si nFET
Si pFET
JL Mode
Lg =3nm
0.3
0.2
0.1
0.0
-2
-1
0
1
2
Drain Voltage (V)
Fig. 8.10 Id–Vg of 3-nm gate length (Lg) for n-type and p-type Si bulk FinFET operating in JL
mode with SS and DIBL values shown inset and Id–Vd of 3-nm gate length (Lg) for n-type and
p-type Si bulk FinFET operating in JL mode, with overdrive voltage |Vov| = |Vg − Vth| [3]
290
8
Extremely Scaled Si and Ge to Lg = 3 nm FinFETs …
-3
10
-4
10
-5
10
-6
10
-7
10
-8
10
-9
10
Vds =-0.7V
Vds =-0.05V
Si nFET
Si pFET
Vds = 0.7V
AC Mode
Lg =3nm
Vds =0.05V
Si pFET SS :
67.65 mV/dec
Si nFET SS :
78.79 mV/dec
Si pFET DIBL :
31.89mv/V
Si nFET DIBL :
16.17 mv/V
IVg
Drain Current (mA/µm)
Drain Current (A/µ m)
0.5
10
-10
-1.0
-0.5
0.0
0.5
Si nFET
Si pFET
0.4
AC Mode
L g =3nm
0.3
0.2
0.1
0.0
1.0
Vth I= 0.4 V to 0.8 V
Step = 0.2 V
-2
-1
Gate Voltage (V)
0
1
2
Drain Voltage (V)
Fig. 8.11 Id–Vg of 3-nm gate length (Lg) for n-type and p-type Si bulk FinFET operating in AC
mode with SS and DIBL values shown inset and Id–Vd of 3-nm gate length (Lg) for n-type and
p-type Si bulk FinFET operating in AC mode, with overdrive voltage |Vov| = |Vg − Vth| [3]
-3
10
-4
10
-5
10
-6
10
-7
10
-8
10
-9
10
Vds =-0.7V
Vds =-0.05V
Si nFET
Si pFET
Vds = 0.7V
IM Mode
Lg =3nm
Vds =0.05V
Si pFET SS :
67.63 mV/dec
Si nFET SS :
78.74 mV/dec
Si pFET DIBL :
29.80mv/V
Si nFET DIBL :
16.04 mv/V
IVg
Drain Current (mA/µm)
Drain Current (A/µ m)
0.5
10
-10
-1.0
-0.5
0.0
0.5
Gate Voltage (V)
1.0
Vth I= 0.4 V to 0.8 V
Step = 0.2 V
Si nFET
Si pFET
0.4
IM Mode
Lg =3nm
0.3
0.2
0.1
0.0
-2
-1
0
1
2
Drain Voltage (V)
Fig. 8.12 Id–Vg of 3-nm gate length (Lg) for n-type and p-type Si bulk FinFET operating in IM
with SS and DIBL values shown inset and Id–Vd of 3-nm gate length (Lg) for n-type and p-type Si
bulk FinFET operating in IM, with overdrive voltage |Vov| = |Vg − Vth| [3]
It is noteworthy that the off-state current is all low in IM, AC, and JL modes of
Si bulk FinFET owing to extensively scaled nanoﬁn.
Right-hand side plots of Figs. 8.10, 8.11, and 8.12 show the output characteristic
curves of Si FinFET. It is very clear that simulated IM and AC devices have almost
similar Id–Vd output characteristic curves.
Figure 8.13a, b compares on-state (Vgs = 1 V) and off-state (Vgs = 1 mV)
electron density distribution at the 3D cross sections of the 3-nm nanoﬁn n-type Si
bulk JL-FinFET. The conduction path is located at the middle of the nanoﬁn as
expected. Figure 8.13c–f compares on-state (Vgs = 1 V) and off-state (Vgs = 1 mV)
8.3 Study of Silicon Lg = 3 nm Bulk IM, AC …
291
Table 8.1 Important numerical values of simulated 3-nm gate length IM, AC, and JL Si bulk
FinFETs [3]
Device mode
Junctionless
Accumulation
Inversion
Work function (eV)
N: 4.55
P: 4.60
N: 0.3057
P: −0.2969
N: 77.37
P: 62.28
N: 26.80
P: 40.20
N: 2.32 Â 10−4
P: 2.26 Â 10−4
N: 4.40
P: 4.80
N: 0.2987
P: −0.2987
N: 78.79
P: 67.65
N: 16.17
P: 31.89
N: 2.54 Â 10−4
P: 2.24 Â 10−4
N: 4.40
P: 4.80
N: 0.3000
P: −0.3019
N: 78.74
P: 67.63
N: 16.04
P: 29.80
N: 2.522 Â 10−4
P: 2.240 Â 10−4
Vth (*0.31 V)
SS (mV/dec)
DIBL (mv/V)
Ion (A/lm)
electron density distribution at the 3D cross sections of the 3-nm nanoﬁn n-type Si
bulk IM-FinFET and AC-FinFET, respectively. Notably, the on-state and off-state
results of 3-D eDensity distribution from quantum transport simulation demonstrate
that the device can be scaled down to a physical limit of 3-nm node. The current
conduction in all three (JL, AC, and IM) modes is almost similar because the
carriers fully occupy 3-nm nanoﬁn cross section. The electrons are more concentrated at the middle topside of channel in IM, AC, and JL bulk FinFET as better
controllability by gate is achieved with Lg = Fw = Fh = 3 nm.
In summary, we have performed various analyses in the 3-nm gate length bulk
silicon FinFET operating in inversion-mode (IM), accumulation-mode (AC), and
junctionless-mode (JL). The observed transfer characteristics, output characteristics,
and electron density distribution results of the 3D quantum transport device simulation reveal the fact that all the three IM, AC, and JL modes of operation are
perfectly feasible even at 3-nm gate length. Thus, it enables the bulk FinFET
devices to be scaled down to its least possible physical limits obeying Moore’s
scaling law.
8.4
Study of Germanium Lg = 3-nm Bulk FinFET
In this section, the Synopsys Sentaurus TCAD 2014 version 3D device simulation
is used to show the performances of n-type and p-type 3-nm bulk Ge FinFET of
IM-FET, AC-FET, and JL—FET. The simulated bulk Ge FinFET device exhibits
better short-channel characteristics, including drain-induced barrier lowering
(DIBL < 10 mV/V) and subthreshold slope (SS * 64 mV/dec). Electron density
distributions in on-state and off-state also show that the simulated devices have
better Ion/ Ioff ratios.
Extremely Scaled Si and Ge to Lg = 3 nm FinFETs …
8
(a)
(b)
Z
3
(#/cm )
G
1e+20
X
G
6e+19
4e+19
)
He
G
2e+14
2e+14
G
2e+14
1e+14
ity
Electron Dens
3
(#/cm )
m
ht
1.5
1e+14
1e+14
4e+19
(n
m)
ht
0.5
(f)
G
3
G
8.0e+19
1.6e+14
G
1.4e+14
1.2e+14
1.0e+14
6.0e+19
8.0e+13
)
m
(n
0.0
3.0
2.5
2.0
1.5
1.0
0.5
0.0
2.5
2.0
Fin W 1.5 1.0
0.5
id
S u b s th (n m )
trate
ht
1.0
2.0e+13
ig
1.5
4.0e+13
He
2.0
0.5
Fin W
id
(Sub th (nm)
strat
e)
6.0e+13
n
2.5
3.0
2.5
2.0
1.5
1.0
0.5
0.0
He
ig
ht
(n
m
)
2.0e+19
Fi
n
4.0e+19
0.0
2.0
Fin W 1.5 1.0
id
(S u bs t h ( n m )
t r at e )
Fi
1.0e+20
2.5
1.8e+14
ity
Electron Dens
1.2e+20
(#/cm )
G
1.4e+20
3.0
2.5
2.0
1.5
1.0
0.5
0.0
Fi
nH
eig
m
(n
ht
ig
0.5
He
2.0
Fin W 1.5 1.0
id
( S u b th ( n m )
s tr a t
e)
n
2.5
6e+13
4e+13
2e+13
0
Fi
0
3.0
2.5
2.0
1.5
1.0
0.5
0.0
)
8e+13
2e+19
(e)
3
(n
Fi
n
G
6e+19
ity (#/cm )
2.0
(d)
G
8e+19
2.5
1.0
Fin W
0.5
id
(S u b th (n m )
s t r a te
)
1e+20
ity
Electron Dens
3
(#/cm )
(c)
0
n
1.0
Fi
1.5
3.0
2.5
2.0
1.5
1.0
0.5
0.0
2e+14
ig
nm
)
2.0
t(
2.5
0.5
Fin W
id
(Subs th (nm)
trate)
Electron Dens
G
4e+14
3.0
2.5
2.0
1.5
1.0
0.5
0.0
2e+19
0
G
8e+14
6e+14
He
ig
h
Electron Density
8e+19
1e+15
ity
Electron Dens
Y
3
(#/cm )
292
Fig. 8.13 3D mesh plot for electron density distributions in the 3-nm gate length (Lg) n-type Si
bulk FinFET in (a) JL on-state (Vgs = 1 V) and (b) JL off-state (Vgs = 1 mV); (c) IM on-state and
(d) IM off-state; and (e) AC on-state and (f) AC off-state [3]
Simulation Method
The simulated device structure and the table of important parameters used in the
device simulation are given in Fig. 8.14. We applied equivalent oxide thickness
(EOT) of 0.3 nm. The gate length (Lg) is 3 nm, and the Fin width (Fw) and the Fin
height (Fh) are also the same (Fw = Fh = 3 nm). The doping concentrations of